Band Gap Opening of Graphene by Noncovalent π-π ...file.scirp.org/pdf/Graphene_ ·...
Embed Size (px)
Transcript of Band Gap Opening of Graphene by Noncovalent π-π ...file.scirp.org/pdf/Graphene_ ·...
Graphene, 2013, 2, 102-108 http://dx.doi.org/10.4236/graphene.2013.23015 Published Online July 2013 (http://www.scirp.org/journal/graphene)
Band Gap Opening of Graphene by Noncovalent - Interaction with Porphyrins
Arramel1*, Andres Castellanos-Gomez1,2, Bart Jan van Wees1 1Physics of Nanodevices, Zernike Institute for Advanced Materials, University of Groningen,
Groningen, The Netherlands 2Kavli Institute of Nanoscience, Delft University of Technology, Delft, The Netherlands
Received May 12, 2013; revised June 18, 2013; accepted July 5, 2013
Copyright 2013 Arramel et al. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.
ABSTRACT Graphene has been recognized as a promising 2D material with many new properties. However, pristine graphene is gapless which hinders its direct application towards graphene-based semiconducting devices. Recently, various ways have been proposed to overcome this problem. In this study, we report a robust method to open a gap in graphene via noncovalent functionalization with porphyrin molecules. Two type of porphyrins, namely, iron protoporphyrin (FePP) and zinc protoporphryin (ZnPP) were independently physisorbed on graphene grown on nickel by chemical vapour de- position (CVD) resulting in a bandgap opening in graphene. Using a statistical analysis of scanning tunneling spectros- copy (STS) measurements, we demonstrated that the magnitude of the band gap depends on the type of deposited por- phyrin molecule.The - stacking of FePP on graphene yielded a considerably larger band gap value (0.45 eV) than physisorbed ZnPP (0.23 eV). We proposed that the origin of different band gap value is governed due to the metallic character of the respective porphyrin. Keywords: Band Gap; Graphene; Scanning Tunneling Spectroscopy; Porphyrins; - Stacking
1. Introduction The development of novel techniques to produce highly crystalline monolayer graphene on the surface of transi- tion metals is bringing graphene-based applications a step closer [1-6]. However, the absence of band gap around the Fermi level in graphene is hampering its ap- plication in nanoelectronic and photonic devices , since an energy gap is necessary to fabricate field effect transistors with a large current on-off ratio [7,8]. This fact has motivated the study of different methods to open a band gap in graphene. The band structure of graphene is mainly governed by its special electronic properties where and * bands are crossing at the so called Dirac neutrality point. The opening of a gap in graphene can be realized by breaking its symmetry in various approaches: defect formation , chemical dopants [10-12], electric fields [13-15], and interaction with gases .
The noncovalent stacking of aromatic organic molecu- les on graphene through - interaction is emerging as a promising route to tailor the electronic properties of gra- phene , motivated by the study of the interaction be-
tween large aromatic molecules and graphene [18-20]. Among all possible aromatic molecules, porphyrins are of primary interest in molecular electronics due to their rich electronic/photonic properties (including charge tran- sport, energy transfer, light absorption or emission) . Individual porphyrin molecules physorbed on different substrates have shown that their structure can be well- resolved using scanning tunneling microscopy (STM) [22-24]. In particular, metalloporphyrins (with a metal ion at the central part of the porphyrin) have attracted much interest due to their peculiar electronic properties . However, a microscopic knowledge of the topo- graphic and the local electronic structure of physisorbed porphyrin molecules on monolayer graphene is still lack- ing.
In this work the - stacking of porphryins on graph- ene and its effect on the electronic properties of graphene is investigated. Two different types of porphyrin mole- cules, namely, iron protoporphyrin and zinc porphryins were physisorbed on CVD graphene grown on nickel. By means of a systematic statistical analysis of scanning tunnelling spectroscopy measurements, we probe the opening of an energy bandgap in graphene in the vicinity *Corresponding author.
Copyright 2013 SciRes. Graphene
ARRAMEL ET AL. 103
of physisorbed porphyrins. Although optical experiments (photo electron spectroscopy or UV-VIS experiments) can be useful to probe the electronic properties of a fully functionalized graphene surface, scanning tunneling spectroscopy allows one the chance to study even single molecules and to investigate of the electronic properties of the sample with high accuracy and spatial resolution.
2. Experiments STM measurements were carried out using a PicoLE STM (Agilent) equipped with low tunneling current STM scanner head (type: N9501-A) and digital instrument from Agilent Technologies model N960A. STM Tips were obtained by mechanically cutting 0.25 mm Pt0.8Ir0.2 wire (Goodfellow). The STM images were acquired in constant current operating mode, in air at room tempera- ture. Typical scanning parameters to obtain STM images are in the range of 10 to 15 pA with the tip bias voltage ranging from 0.8 to 1.2 V. The STM images were treated by standard flattening procedure without further image processing treatment. The porphyrins were used without any further purification from Aldrich. A solution 1.63 mM of FePP in uvasol grade chloroform was pre- pared. Further, a droplet of 10 L of the porphyrin solu- tion was dropcasted onto CVD-graphene surface and the solvent was left to evaporate for 3h in open air condition. The same procedure was also applied for the deposition of ZnPP.
3. Results and Discussion We have studied and used commercially available gra- phene/multi-layered graphene grown by chemical va- pour deposition on polycrystalline nickel . The as received samples have been first characterized by scan- ning tunnelling microscopy and spectroscopy. Figure 1 shows the STM topography, measured in constant cur- rent mode, of the surface of the CVD graphene on nickel, showing a characteristic rippled structure (a Moir pat- tern) due to mismatching between the graphene and nickel lattices. The topographic line profile, measured along the black line in Figure 1(c), shows the graphene atomic corrugation superimposed to the Moir pattern of graphene (Figure 1(d)). Iron porphyrins (FePP) are then deposited onto the CVD graphene surface by drop cast- ing.
Figure 2(b) shows the STM topography of the CVD graphene surface after the deposition of FePP molecules. There are two main features associated with the presence of FePP molecules on the surface: small and chain-like protuberances (see Figure 2(c)). While chain-like struc- tures present typical lengths ranging from 4.5 nm to 7 nm and 0.6 nm in height, higher resolution images reveals that the small protuberances have a star-like shape with
Figure 1. A representative STM image of pristine CVD- graphene probed in ambient condition; (a) 160 160 nm2 STM image covered with single layer of graphene (It = 0.1 nA; V = 0.5 V; Z-scale = 2.05 nm); (b) Super mesh of single layer graphene decorated with a hexagonal moir feature throughout the entire surface area (It = 0.1 nA; V = 0.3 V; Z-scale = 5.01 ); (c) Carbon atoms arranged in the honey- comb lattice is markedly the evidence of single layer gra- phene on nickel substrate (It = 0.1 nA; V = 0.3 V; Z-scale = 5.01 ); (d) A corresponding cross section profile drawn from a solid black line in Figure 1(c). 0.26 nm in height and approximate dimension of 13 19 (Figure 2(d)). These lateral dimensions are in agreement with the dimensions of a single porphyrin molecule obtained by first principle calculations (16 16 ) . The resolved six-star shape, however, do not perfectly match to the expected geometrical structure of porphyrin molecules (four-star shape).
The additional features in the observed star shape can be due to the splitting of the local density of the state (LDOS) of one phenyl ring. Another interesting finding is that FePP molecules are preferable physisorbed at the valleys of the Moir structure of graphene (Figure 2(c)). The origin of the chain-like structures is possibly driven by a noncovalent interaction created between the next neighboring FePP extended up to few nanometers. To evaluate further the effect of the molecule-substrate (MS) interaction, we present another example of self-assem- bled porphyrin on graphene using Zincporphyrin (ZnPP) molecules with a weaker interaction with the graphene surface . The molecular structure is illustrated in Figure 2(e). We deposited the ZnPP in a similar way as the FePP. The ZnPP molecule is mainly constructed of a zinc metal at the central propyrins backbone which is a rather weak transition metal in comparison to Fe. Inter-
Copyright 2013 SciRes. Graphene
ARRAMEL ET AL.
Copyright 2013 SciRes. Graphene
Figure 2. Single molecule detection of porphyrins on CVD-grown graphene; (a) 5,10,15,20-Tetraphenyl-21H,23H-porphine iron(III) chloride (abbreviated as FePP); (b) Porphyrin molecules decorating the terraces of single layer graphene (It = 0.1 nA; V = 0.5 V). FePP can be found at the valleys of the Moir pattern of graphene; (c) Single porphyrin molecules with star-like shape were observed at the vicinity of hills of the rippled structure of graphene on Ni; (d) Topographic line profile alongthe